#------------------------------------------------------------------------------
#$Date: 2017-10-28 08:17:16 +0300 (Sat, 28 Oct 2017) $
#$Revision: 202402 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/22/94/7229417.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7229417
loop_
_publ_author_name
'Bao, Xinjian'
'Liu, Xiaoyang'
'Liu, Xi'
_publ_section_title
;
 High-pressure synthesis, crystal structure and photoluminescence
 properties of a new terbium silicate: Na2Tb1.08Ca2.92Si6O18H0.8
;
_journal_issue                   79
_journal_name_full               'RSC Adv.'
_journal_page_first              50195
_journal_paper_doi               10.1039/C7RA10182A
_journal_volume                  7
_journal_year                    2017
_chemical_formula_sum            'Ca2.92 H0.8 Na2 O18 Si6 Tb1.08'
_chemical_formula_weight         792.2
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2017-09-12 deposited with the CCDC.
2017-10-23 downloaded from the CCDC.
;
_cell_angle_alpha                102.381(5)
_cell_angle_beta                 95.387(6)
_cell_angle_gamma                90.552(6)
_cell_formula_units_Z            1
_cell_length_a                   7.056(3)
_cell_length_b                   7.075(3)
_cell_length_c                   8.029(3)
_cell_measurement_reflns_used    1416
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.34
_cell_measurement_theta_min      2.61
_cell_volume                     389.6(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Bruker Smart Apex II Quazar CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0109
_diffrn_reflns_av_sigmaI/netI    0.0203
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -3
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            2059
_diffrn_reflns_theta_full        25.34
_diffrn_reflns_theta_max         25.34
_diffrn_reflns_theta_min         2.61
_exptl_absorpt_coefficient_mu    6.478
_exptl_absorpt_correction_T_max  0.723
_exptl_absorpt_correction_T_min  0.542
_exptl_absorpt_correction_type   multi-scans
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.377
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             380
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.898
_refine_diff_density_min         -0.978
_refine_diff_density_rms         0.212
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.015
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     141
_refine_ls_number_reflns         1416
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.014
_refine_ls_R_factor_all          0.0506
_refine_ls_R_factor_gt           0.0502
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+19.9119P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1186
_refine_ls_wR_factor_ref         0.1188
_reflns_number_gt                1399
_reflns_number_total             1416
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c7ra10182a2.cif
_cod_data_source_block           92-4-15r2
_cod_original_cell_volume        389.6(2)
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7229417
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ca1 Ca 0.14025(19) 0.5793(2) 0.34642(17) 0.0097(3) Uani 0.875 1 d P
Tb1 Tb 0.14025(19) 0.5793(2) 0.34642(17) 0.0097(3) Uani 0.125 1 d P
Ca2 Ca 0.14971(11) 0.09669(12) 0.35501(10) 0.0086(2) Uani 0.585 1 d P
Tb2 Tb 0.14971(11) 0.09669(12) 0.35501(10) 0.0086(2) Uani 0.415 1 d P
Na1 Na 0.3399(7) 0.7641(7) 0.0599(6) 0.0277(10) Uani 1 1 d .
H1 H 0.5253 0.6903 0.4030 0.033 Uiso 0.4 1 d PRD
O1 O 0.4533(11) 0.6391(12) 0.3150(11) 0.0234(17) Uani 1 1 d D
O2 O 0.0495(9) 0.8004(11) 0.1679(9) 0.0158(15) Uani 1 1 d .
O3 O 0.1380(11) 0.2803(10) 0.1485(9) 0.0183(16) Uani 1 1 d .
O4 O 0.1841(10) 0.3941(11) 0.5623(9) 0.0195(16) Uani 1 1 d .
O5 O 0.1760(11) -0.1121(12) 0.5664(9) 0.0239(17) Uani 1 1 d .
O6 O 0.2802(10) 0.0387(10) 0.8981(9) 0.0170(15) Uani 1 1 d .
O7 O 0.5420(10) -0.0161(11) 0.6808(10) 0.0191(16) Uani 1 1 d .
O8 O 0.3802(10) -0.3082(10) 0.7695(9) 0.0176(15) Uani 1 1 d .
O9 O 0.2783(11) -0.5921(10) 0.8952(9) 0.0188(16) Uani 1 1 d .
Si1 Si 0.3415(4) -0.0983(4) 0.7197(3) 0.0103(5) Uani 1 1 d .
Si2 Si 0.3415(4) -0.5400(4) 0.7176(4) 0.0128(6) Uani 1 1 d .
Si3 Si -0.1509(4) 0.7670(4) 0.0531(3) 0.0110(6) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Ca1 O3 91.3(3) . .
O1 Ca1 O4 99.1(3) . .
O3 Ca1 O4 85.9(3) . .
O1 Ca1 O2 89.2(3) . .
O3 Ca1 O2 102.8(2) . .
O4 Ca1 O2 167.9(3) . .
O1 Ca1 O4 163.5(3) . 2_566
O3 Ca1 O4 105.1(3) . 2_566
O4 Ca1 O4 82.4(3) . 2_566
O2 Ca1 O4 87.1(2) . 2_566
O1 Ca1 O5 84.1(3) . 1_565
O3 Ca1 O5 174.2(3) . 1_565
O4 Ca1 O5 91.3(3) . 1_565
O2 Ca1 O5 80.8(3) . 1_565
O4 Ca1 O5 79.5(3) 2_566 1_565
O1 Ca1 Na1 48.5(2) . .
O3 Ca1 Na1 86.3(2) . .
O4 Ca1 Na1 146.4(2) . .
O2 Ca1 Na1 44.16(18) . .
O4 Ca1 Na1 131.14(19) 2_566 .
O5 Ca1 Na1 93.4(2) 1_565 .
O1 Ca1 Si2 162.7(2) . 2_556
O3 Ca1 Si2 86.0(2) . 2_556
O4 Ca1 Si2 97.76(19) . 2_556
O2 Ca1 Si2 74.79(17) . 2_556
O4 Ca1 Si2 25.52(18) 2_566 2_556
O5 Ca1 Si2 99.39(19) 1_565 2_556
Na1 Ca1 Si2 114.24(10) . 2_556
O1 Ca1 Ca2 100.6(2) . .
O3 Ca1 Ca2 42.18(17) . .
O4 Ca1 Ca2 43.92(19) . .
O2 Ca1 Ca2 143.12(18) . .
O4 Ca1 Ca2 91.87(18) 2_566 .
O5 Ca1 Ca2 135.18(19) 1_565 .
Na1 Ca1 Ca2 123.16(10) . .
Si2 Ca1 Ca2 88.87(6) 2_556 .
O1 Ca1 Si2 81.7(2) . 1_565
O3 Ca1 Si2 101.80(19) . 1_565
O4 Ca1 Si2 23.37(18) . 1_565
O2 Ca1 Si2 153.93(18) . 1_565
O4 Ca1 Si2 94.66(18) 2_566 1_565
O5 Ca1 Si2 74.00(19) 1_565 1_565
Na1 Ca1 Si2 129.97(10) . 1_565
Si2 Ca1 Si2 115.53(6) 2_556 1_565
Ca2 Ca1 Si2 62.90(5) . 1_565
O1 Ca1 Si3 109.7(2) . .
O3 Ca1 Si3 90.02(19) . .
O4 Ca1 Si3 151.04(19) . .
O2 Ca1 Si3 23.76(17) . .
O4 Ca1 Si3 71.00(18) 2_566 .
O5 Ca1 Si3 94.93(19) 1_565 .
Na1 Ca1 Si3 61.49(10) . .
Si2 Ca1 Si3 53.32(7) 2_556 .
Ca2 Ca1 Si3 123.81(6) . .
Si2 Ca1 Si3 163.56(8) 1_565 .
O7 Ca2 O3 92.8(3) 2_656 .
O7 Ca2 O2 88.9(3) 2_656 1_545
O3 Ca2 O2 96.5(3) . 1_545
O7 Ca2 O4 102.7(3) 2_656 .
O3 Ca2 O4 87.0(2) . .
O2 Ca2 O4 167.7(2) 1_545 .
O7 Ca2 O5 164.7(3) 2_656 2_556
O3 Ca2 O5 102.0(3) . 2_556
O2 Ca2 O5 85.6(2) 1_545 2_556
O4 Ca2 O5 82.2(3) . 2_556
O7 Ca2 O5 84.3(3) 2_656 .
O3 Ca2 O5 176.6(3) . .
O2 Ca2 O5 81.8(3) 1_545 .
O4 Ca2 O5 95.3(3) . .
O5 Ca2 O5 80.8(3) 2_556 .
O7 Ca2 Na1 48.3(2) 2_656 1_545
O3 Ca2 Na1 84.4(2) . 1_545
O2 Ca2 Na1 43.21(18) 1_545 1_545
O4 Ca2 Na1 149.0(2) . 1_545
O5 Ca2 Na1 128.7(2) 2_556 1_545
O5 Ca2 Na1 92.4(2) . 1_545
O7 Ca2 Ca1 104.26(19) 2_656 .
O3 Ca2 Ca1 43.21(18) . .
O2 Ca2 Ca1 137.07(18) 1_545 .
O4 Ca2 Ca1 44.05(18) . .
O5 Ca2 Ca1 89.4(2) 2_556 .
O5 Ca2 Ca1 139.29(18) . .
Na1 Ca2 Ca1 123.32(9) 1_545 .
O7 Ca2 Si1 160.2(2) 2_656 2_556
O3 Ca2 Si1 83.1(2) . 2_556
O2 Ca2 Si1 72.45(17) 1_545 2_556
O4 Ca2 Si1 96.42(18) . 2_556
O5 Ca2 Si1 24.46(18) 2_556 2_556
O5 Ca2 Si1 99.13(19) . 2_556
Na1 Ca2 Si1 111.91(10) 1_545 2_556
Ca1 Ca2 Si1 85.94(5) . 2_556
O7 Ca2 Si3 108.6(2) 2_656 1_545
O3 Ca2 Si3 85.15(19) . 1_545
O2 Ca2 Si3 22.26(17) 1_545 1_545
O4 Ca2 Si3 148.07(19) . 1_545
O5 Ca2 Si3 69.36(18) 2_556 1_545
O5 Ca2 Si3 94.13(18) . 1_545
Na1 Ca2 Si3 60.49(10) 1_545 1_545
Ca1 Ca2 Si3 119.19(6) . 1_545
Si1 Ca2 Si3 51.91(6) 2_556 1_545
O7 Ca2 Si2 86.1(2) 2_656 1_565
O3 Ca2 Si2 98.86(19) . 1_565
O2 Ca2 Si2 164.09(18) 1_545 1_565
O4 Ca2 Si2 19.90(18) . 1_565
O5 Ca2 Si2 95.27(18) 2_556 1_565
O5 Ca2 Si2 82.70(19) . 1_565
Na1 Ca2 Si2 134.45(10) 1_545 1_565
Ca1 Ca2 Si2 58.83(5) . 1_565
Si1 Ca2 Si2 113.58(7) 2_556 1_565
Si3 Ca2 Si2 164.63(7) 1_545 1_565
O2 Na1 O8 124.2(3) . 1_564
O2 Na1 O1 87.3(3) . .
O8 Na1 O1 136.9(3) 1_564 .
O2 Na1 O7 85.3(3) . 2_666
O8 Na1 O7 137.5(3) 1_564 2_666
O1 Na1 O7 64.7(3) . 2_666
O2 Na1 O6 92.3(3) . 1_564
O8 Na1 O6 63.4(3) 1_564 1_564
O1 Na1 O6 152.8(3) . 1_564
O7 Na1 O6 88.1(3) 2_666 1_564
O2 Na1 O9 96.1(3) . 1_564
O8 Na1 O9 62.4(3) 1_564 1_564
O1 Na1 O9 88.0(3) . 1_564
O7 Na1 O9 152.6(3) 2_666 1_564
O6 Na1 O9 119.1(3) 1_564 1_564
O2 Na1 O6 140.5(3) . 2_666
O8 Na1 O6 85.1(3) 1_564 2_666
O1 Na1 O6 85.9(3) . 2_666
O7 Na1 O6 56.8(2) 2_666 2_666
O6 Na1 O6 77.2(3) 1_564 2_666
O9 Na1 O6 122.5(3) 1_564 2_666
O2 Na1 O9 143.2(3) . 2_656
O8 Na1 O9 85.2(3) 1_564 2_656
O1 Na1 O9 56.6(2) . 2_656
O7 Na1 O9 85.1(3) 2_666 2_656
O6 Na1 O9 122.8(3) 1_564 2_656
O9 Na1 O9 77.5(3) 1_564 2_656
O6 Na1 O9 52.1(2) 2_666 2_656
O2 Na1 Si1 112.2(2) . 1_564
O8 Na1 Si1 31.30(19) 1_564 1_564
O1 Na1 Si1 160.5(3) . 1_564
O7 Na1 Si1 113.9(2) 2_666 1_564
O6 Na1 Si1 32.15(17) 1_564 1_564
O9 Na1 Si1 91.1(2) 1_564 1_564
O6 Na1 Si1 78.20(18) 2_666 1_564
O9 Na1 Si1 104.2(2) 2_656 1_564
O2 Na1 Si2 114.7(3) . 1_564
O8 Na1 Si2 30.52(19) 1_564 1_564
O1 Na1 Si2 113.6(3) . 1_564
O7 Na1 Si2 160.0(3) 2_666 1_564
O6 Na1 Si2 91.3(2) 1_564 1_564
O9 Na1 Si2 31.98(17) 1_564 1_564
O6 Na1 Si2 103.6(2) 2_666 1_564
O9 Na1 Si2 78.47(19) 2_656 1_564
Si1 Na1 Si2 60.46(11) 1_564 1_564
O2 Na1 Ca1 46.6(2) . .
O8 Na1 Ca1 140.1(3) 1_564 .
O1 Na1 Ca1 44.05(19) . .
O7 Na1 Ca1 82.2(2) 2_666 .
O6 Na1 Ca1 138.1(2) 1_564 .
O9 Na1 Ca1 79.1(2) 1_564 .
O6 Na1 Ca1 127.1(2) 2_666 .
O9 Na1 Ca1 96.94(19) 2_656 .
Si1 Na1 Ca1 154.24(17) 1_564 .
Si2 Na1 Ca1 110.78(16) 1_564 .
Si2 O1 Ca1 144.6(5) 2_656 .
Si2 O1 Na1 108.2(4) 2_656 .
Ca1 O1 Na1 87.4(3) . .
Si3 O2 Na1 124.3(4) . .
Si3 O2 Tb2 123.8(4) . 1_565
Na1 O2 Tb2 92.0(3) . 1_565
Si3 O2 Ca2 123.8(4) . 1_565
Na1 O2 Ca2 92.0(3) . 1_565
Tb2 O2 Ca2 0.00(5) 1_565 1_565
Si3 O2 Ca1 119.2(4) . .
Na1 O2 Ca1 89.3(3) . .
Tb2 O2 Ca1 100.2(3) 1_565 .
Ca2 O2 Ca1 100.2(3) 1_565 .
Si3 O3 Ca2 134.4(4) 2_565 .
Si3 O3 Ca1 130.6(4) 2_565 .
Ca2 O3 Ca1 94.6(3) . .
Si2 O4 Ca2 129.2(4) 1_565 .
Si2 O4 Ca1 119.7(4) 1_565 .
Ca2 O4 Ca1 92.0(3) . .
Si2 O4 Ca1 112.2(4) 1_565 2_566
Ca2 O4 Ca1 100.3(3) . 2_566
Ca1 O4 Ca1 97.6(3) . 2_566
Si2 O4 Tb1 112.2(4) 1_565 2_566
Ca2 O4 Tb1 100.3(3) . 2_566
Ca1 O4 Tb1 97.6(3) . 2_566
Ca1 O4 Tb1 0.000(18) 2_566 2_566
Si1 O5 Tb2 116.5(4) . 2_556
Si1 O5 Ca2 116.5(4) . 2_556
Tb2 O5 Ca2 0.00(4) 2_556 2_556
Si1 O5 Ca2 125.9(4) . .
Tb2 O5 Ca2 99.2(3) 2_556 .
Ca2 O5 Ca2 99.2(3) 2_556 .
Si1 O5 Ca1 117.2(4) . 1_545
Tb2 O5 Ca1 98.1(3) 2_556 1_545
Ca2 O5 Ca1 98.1(3) 2_556 1_545
Ca2 O5 Ca1 94.5(3) . 1_545
Si1 O5 Tb1 117.2(4) . 1_545
Tb2 O5 Tb1 98.1(3) 2_556 1_545
Ca2 O5 Tb1 98.1(3) 2_556 1_545
Ca2 O5 Tb1 94.5(3) . 1_545
Ca1 O5 Tb1 0.00(4) 1_545 1_545
Si1 O6 Si3 135.4(5) . 2_566
Si1 O6 Na1 91.4(3) . 1_546
Si3 O6 Na1 129.2(4) 2_566 1_546
Si1 O6 Na1 87.8(3) . 2_666
Si3 O6 Na1 98.3(3) 2_566 2_666
Na1 O6 Na1 102.8(3) 1_546 2_666
Si1 O7 Tb2 143.0(4) . 2_656
Si1 O7 Ca2 143.0(4) . 2_656
Tb2 O7 Ca2 0.00(6) 2_656 2_656
Si1 O7 Na1 106.5(4) . 2_666
Tb2 O7 Na1 88.7(3) 2_656 2_666
Ca2 O7 Na1 88.7(3) 2_656 2_666
Si2 O8 Si1 147.1(5) . .
Si2 O8 Na1 102.6(4) . 1_546
Si1 O8 Na1 101.2(4) . 1_546
Si2 O9 Si3 136.4(5) . 2_556
Si2 O9 Na1 91.4(3) . 1_546
Si3 O9 Na1 128.8(4) 2_556 1_546
Si2 O9 Na1 87.9(3) . 2_656
Si3 O9 Na1 97.1(3) 2_556 2_656
Na1 O9 Na1 102.5(3) 1_546 2_656
O5 Si1 O7 113.8(4) . .
O5 Si1 O8 112.2(4) . .
O7 Si1 O8 107.2(4) . .
O5 Si1 O6 111.1(4) . .
O7 Si1 O6 108.1(4) . .
O8 Si1 O6 103.8(4) . .
O5 Si1 Na1 129.8(3) . 1_546
O7 Si1 Na1 116.2(3) . 1_546
O8 Si1 Na1 47.5(3) . 1_546
O6 Si1 Na1 56.4(3) . 1_546
O5 Si1 Na1 136.7(3) . 2_666
O7 Si1 Na1 46.0(3) . 2_666
O8 Si1 Na1 110.7(3) . 2_666
O6 Si1 Na1 62.7(3) . 2_666
Na1 Si1 Na1 84.79(14) 1_546 2_666
O5 Si1 Ca2 39.0(3) . 2_556
O7 Si1 Ca2 146.4(3) . 2_556
O8 Si1 Ca2 103.3(3) . 2_556
O6 Si1 Ca2 77.4(3) . 2_556
Na1 Si1 Ca2 94.75(11) 1_546 2_556
Na1 Si1 Ca2 132.10(12) 2_666 2_556
O5 Si1 Ca1 39.0(3) . 1_545
O7 Si1 Ca1 108.4(3) . 1_545
O8 Si1 Ca1 78.4(3) . 1_545
O6 Si1 Ca1 140.8(3) . 1_545
Na1 Si1 Ca1 116.70(13) 1_546 1_545
Na1 Si1 Ca1 153.89(11) 2_666 1_545
Ca2 Si1 Ca1 64.36(5) 2_556 1_545
O4 Si2 O8 113.4(4) 1_545 .
O4 Si2 O1 113.5(4) 1_545 2_656
O8 Si2 O1 107.2(4) . 2_656
O4 Si2 O9 112.1(4) 1_545 .
O8 Si2 O9 103.3(4) . .
O1 Si2 O9 106.6(4) 2_656 .
O4 Si2 Na1 131.7(3) 1_545 1_546
O8 Si2 Na1 46.8(3) . 1_546
O1 Si2 Na1 114.6(3) 2_656 1_546
O9 Si2 Na1 56.6(3) . 1_546
O4 Si2 Na1 135.6(3) 1_545 2_656
O8 Si2 Na1 110.4(3) . 2_656
O1 Si2 Na1 44.3(3) 2_656 2_656
O9 Si2 Na1 62.8(3) . 2_656
Na1 Si2 Na1 84.72(15) 1_546 2_656
O4 Si2 Ca1 42.3(3) 1_545 2_556
O8 Si2 Ca1 102.6(3) . 2_556
O1 Si2 Ca1 148.4(3) 2_656 2_556
O9 Si2 Ca1 76.0(3) . 2_556
Na1 Si2 Ca1 93.39(11) 1_546 2_556
Na1 Si2 Ca1 131.55(12) 2_656 2_556
O4 Si2 Tb1 42.3(3) 1_545 2_556
O8 Si2 Tb1 102.6(3) . 2_556
O1 Si2 Tb1 148.4(3) 2_656 2_556
O9 Si2 Tb1 76.0(3) . 2_556
Na1 Si2 Tb1 93.39(11) 1_546 2_556
Na1 Si2 Tb1 131.55(12) 2_656 2_556
Ca1 Si2 Tb1 0.00(5) 2_556 2_556
O4 Si2 Ca1 36.9(3) 1_545 1_545
O8 Si2 Ca1 81.0(3) . 1_545
O1 Si2 Ca1 109.9(3) 2_656 1_545
O9 Si2 Ca1 140.1(3) . 1_545
Na1 Si2 Ca1 118.34(12) 1_546 1_545
Na1 Si2 Ca1 153.32(12) 2_656 1_545
Ca1 Si2 Ca1 64.47(6) 2_556 1_545
Tb1 Si2 Ca1 64.47(6) 2_556 1_545
O4 Si2 Ca2 30.9(3) 1_545 1_545
O8 Si2 Ca2 139.1(3) . 1_545
O1 Si2 Ca2 86.0(3) 2_656 1_545
O9 Si2 Ca2 109.8(3) . 1_545
Na1 Si2 Ca2 157.17(13) 1_546 1_545
Na1 Si2 Ca2 105.85(11) 2_656 1_545
Ca1 Si2 Ca2 64.34(6) 2_556 1_545
Tb1 Si2 Ca2 64.34(6) 2_556 1_545
Ca1 Si2 Ca2 58.26(6) 1_545 1_545
O3 Si3 O2 115.2(4) 2_565 .
O3 Si3 O6 108.1(4) 2_565 2_566
O2 Si3 O6 109.5(4) . 2_566
O3 Si3 O9 109.4(4) 2_565 2_556
O2 Si3 O9 110.1(4) . 2_556
O6 Si3 O9 104.0(4) 2_566 2_556
O3 Si3 Na1 82.0(3) 2_565 .
O2 Si3 Na1 33.2(3) . .
O6 Si3 Na1 125.8(3) 2_566 .
O9 Si3 Na1 123.0(3) 2_556 .
O3 Si3 Ca1 125.1(3) 2_565 .
O2 Si3 Ca1 37.0(3) . .
O6 Si3 Ca1 124.8(3) 2_566 .
O9 Si3 Ca1 73.4(3) 2_556 .
Na1 Si3 Ca1 56.80(9) . .
O3 Si3 Ca2 125.2(3) 2_565 1_565
O2 Si3 Ca2 34.0(3) . 1_565
O6 Si3 Ca2 75.7(3) 2_566 1_565
O9 Si3 Ca2 122.9(3) 2_556 1_565
Na1 Si3 Ca2 57.43(9) . 1_565
Ca1 Si3 Ca2 63.00(6) . 1_565
O3 Si3 Ca1 29.8(3) 2_565 2_565
O2 Si3 Ca1 113.8(3) . 2_565
O6 Si3 Ca1 130.2(3) 2_566 2_565
O9 Si3 Ca1 83.3(3) 2_556 2_565
Na1 Si3 Ca1 84.13(10) . 2_565
Ca1 Si3 Ca1 104.72(8) . 2_565
Ca2 Si3 Ca1 140.65(9) 1_565 2_565
O3 Si3 Ca2 27.2(3) 2_565 2_565
O2 Si3 Ca2 114.4(3) . 2_565
O6 Si3 Ca2 83.8(3) 2_566 2_565
O9 Si3 Ca2 129.0(3) 2_556 2_565
Na1 Si3 Ca2 86.15(9) . 2_565
Ca1 Si3 Ca2 141.48(9) . 2_565
Ca2 Si3 Ca2 107.95(7) 1_565 2_565
Ca1 Si3 Ca2 56.81(5) 2_565 2_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ca1 O1 2.292(8) .
Ca1 O3 2.357(7) .
Ca1 O4 2.387(7) .
Ca1 O2 2.391(7) .
Ca1 O4 2.464(8) 2_566
Ca1 O5 2.490(8) 1_565
Ca1 Na1 3.294(5) .
Ca1 Si2 3.389(3) 2_556
Ca1 Ca2 3.431(2) .
Ca1 Si2 3.452(3) 1_565
Ca1 Si3 3.466(3) .
Ca2 O7 2.283(7) 2_656
Ca2 O3 2.311(7) .
Ca2 O2 2.361(7) 1_545
Ca2 O4 2.381(8) .
Ca2 O5 2.437(8) 2_556
Ca2 O5 2.473(8) .
Ca2 Na1 3.349(5) 1_545
Ca2 Si1 3.462(3) 2_556
Ca2 Si3 3.512(3) 1_545
Ca2 Si2 3.591(3) 1_565
Na1 O2 2.295(8) .
Na1 O8 2.323(9) 1_564
Na1 O1 2.470(10) .
Na1 O7 2.502(9) 2_666
Na1 O6 2.576(9) 1_564
Na1 O9 2.594(9) 1_564
Na1 O6 2.967(9) 2_666
Na1 O9 2.990(9) 2_656
Na1 Si1 3.091(5) 1_564
Na1 Si2 3.107(6) 1_564
O1 Si2 1.634(8) 2_656
O2 Si3 1.600(7) .
O2 Tb2 2.361(7) 1_565
O2 Ca2 2.361(7) 1_565
O3 Si3 1.593(7) 2_565
O4 Si2 1.576(8) 1_565
O4 Ca1 2.464(8) 2_566
O4 Tb1 2.464(8) 2_566
O5 Si1 1.602(8) .
O5 Tb2 2.437(8) 2_556
O5 Ca2 2.437(8) 2_556
O5 Ca1 2.490(8) 1_545
O5 Tb1 2.490(8) 1_545
O6 Si1 1.645(7) .
O6 Si3 1.654(7) 2_566
O6 Na1 2.576(9) 1_546
O6 Na1 2.967(9) 2_666
O7 Si1 1.606(7) .
O7 Tb2 2.283(7) 2_656
O7 Ca2 2.283(7) 2_656
O7 Na1 2.502(9) 2_666
O8 Si2 1.617(8) .
O8 Si1 1.637(7) .
O8 Na1 2.323(9) 1_546
O9 Si2 1.646(7) .
O9 Si3 1.667(7) 2_556
O9 Na1 2.594(9) 1_546
O9 Na1 2.990(9) 2_656
Si1 Na1 3.091(5) 1_546
Si1 Na1 3.336(6) 2_666
Si1 Ca2 3.462(3) 2_556
Si1 Ca1 3.523(3) 1_545
Si2 O4 1.576(8) 1_545
Si2 O1 1.634(8) 2_656
Si2 Na1 3.107(6) 1_546
Si2 Na1 3.360(6) 2_656
Si2 Ca1 3.389(3) 2_556
Si2 Tb1 3.389(3) 2_556
Si2 Ca1 3.452(3) 1_545
Si2 Ca2 3.591(3) 1_545
Si3 O3 1.593(7) 2_565
Si3 O6 1.654(7) 2_566
Si3 O9 1.667(7) 2_556
Si3 Ca2 3.512(3) 1_565
Si3 Ca1 3.602(3) 2_565
Si3 Ca2 3.610(3) 2_565
